#------------------------------------------------------------------------------
#$Date: 2020-03-05 01:43:09 +0200 (Thu, 05 Mar 2020) $
#$Revision: 248862 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/13/43/4134336.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4134336
loop_
_publ_author_name
'Guo, Shu'
'Zhong, Ruidan'
'Wang, Wei'
'Tao, Jing'
'Ni, Danrui'
'Cava, Robert J.'
_publ_section_title
;
 K₃Ir₂O₆ and
 K<sub>16.3</sub>Ir₈O₃₀, Low dimensional Iridates
 with Infinite IrO₆ Chains.
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_paper_doi               10.1021/jacs.0c00849
_journal_year                    2020
_chemical_formula_moiety         'Ir2 K3 O6'
_chemical_formula_sum            'Ir2 K3 O6'
_chemical_formula_weight         597.70
_space_group_crystal_system      trigonal
_space_group_IT_number           148
_space_group_name_Hall           '-R 3'
_space_group_name_H-M_alt        'R -3 :H'
_atom_sites_solution_hydrogens   None
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             2020-01-20
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            6
_cell_length_a                   10.7907(7)
_cell_length_b                   10.7907(7)
_cell_length_c                   10.5055(7)
_cell_measurement_reflns_used    2441
_cell_measurement_temperature    100
_cell_measurement_theta_max      33.16
_cell_measurement_theta_min      3.78
_cell_volume                     1059.37(12)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL (Sheldrick, 2008)'
_computing_structure_solution    'XS (Sheldrick, 2008)'
_diffrn_ambient_temperature      100
_diffrn_detector                 'Bruker APEX2 area detector'
_diffrn_detector_area_resol_mean 7.9
_diffrn_detector_type            'CCD area detector'
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_device_type  'Bruker SMART APEX2 area detector'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_radiation_monochromator  'mirror optics'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0245
_diffrn_reflns_av_unetI/netI     0.0153
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            6766
_diffrn_reflns_theta_full        33.18
_diffrn_reflns_theta_max         33.18
_diffrn_reflns_theta_min         2.92
_diffrn_source                   'microfocus sealed X-ray tube'
_diffrn_source_type              'Incoatec I\ms'
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    39.389
_exptl_absorpt_correction_T_max  0.7465
_exptl_absorpt_correction_T_min  0.3349
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1259 before and 0.0244 after correction.
The Ratio of minimum to maximum transmission is 0.4486.
The λ/2 correction factor is Not present.
;
_exptl_crystal_colour            black
_exptl_crystal_colour_primary    black
_exptl_crystal_density_diffrn    5.621
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             1554
_exptl_crystal_size_max          0.137
_exptl_crystal_size_mid          0.064
_exptl_crystal_size_min          0.036
_refine_diff_density_max         1.265
_refine_diff_density_min         -1.773
_refine_diff_density_rms         0.292
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.062
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     36
_refine_ls_number_reflns         899
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.062
_refine_ls_R_factor_all          0.0295
_refine_ls_R_factor_gt           0.0175
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0139P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0314
_refine_ls_wR_factor_ref         0.0344
_reflns_number_gt                721
_reflns_number_total             899
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja0c00849_si_002.cif
_cod_data_source_block           190915_ki_800_100_0m
_cod_original_sg_symbol_H-M      'R -3'
_cod_database_code               4134336
_olex2_refinement_description
;
1. Twinned data refinement
 Scales: 0.5956(19)
 0.4044(19)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 'x, y, z'
2 '-y, x-y, z'
3 '-x+y, -x, z'
4 'x+2/3, y+1/3, z+1/3'
5 '-y+2/3, x-y+1/3, z+1/3'
6 '-x+y+2/3, -x+1/3, z+1/3'
7 'x+1/3, y+2/3, z+2/3'
8 '-y+1/3, x-y+2/3, z+2/3'
9 '-x+y+1/3, -x+2/3, z+2/3'
10 '-x, -y, -z'
11 'y, -x+y, -z'
12 'x-y, x, -z'
13 '-x+2/3, -y+1/3, -z+1/3'
14 'y+2/3, -x+y+1/3, -z+1/3'
15 'x-y+2/3, x+1/3, -z+1/3'
16 '-x+1/3, -y+2/3, -z+2/3'
17 'y+1/3, -x+y+2/3, -z+2/3'
18 'x-y+1/3, x+2/3, -z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_disorder_assembly
_atom_site_disorder_group
_atom_site_site_symmetry_order
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Ir1 Ir 0.0000 0.0000 0.0000 0.00294(7) Uani 1 d . . 6 S T P
Ir2 Ir 0.0000 0.0000 0.5000 0.00203(7) Uani 1 d . . 6 S T P
Ir3 Ir 0.0000 0.0000 0.24960(2) 0.00277(6) Uani 1 d . . 3 S T P
K1 K 0.03790(9) 0.30956(8) 0.17563(9) 0.00662(13) Uani 1 d . . 1 . . .
O1 O 0.1503(2) 0.1288(2) 0.1237(2) 0.0048(5) Uani 1 d . . 1 . . .
O2 O 0.0286(3) 0.1524(2) 0.3745(2) 0.0046(5) Uani 1 d . . 1 . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ir Ir -1.4442 7.9887 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Ir3 Ir1 Ir3 180.0 10 . ?
Ir3 Ir1 K1 120.314(14) 10 . ?
Ir3 Ir1 K1 59.686(14) . 3 ?
Ir3 Ir1 K1 120.314(14) . 12 ?
Ir3 Ir1 K1 59.686(14) . . ?
Ir3 Ir1 K1 59.686(14) 10 12 ?
Ir3 Ir1 K1 59.686(14) 10 10 ?
Ir3 Ir1 K1 120.314(14) . 10 ?
Ir3 Ir1 K1 120.314(14) 10 3 ?
K1 Ir1 K1 96.769(19) . 3 ?
K1 Ir1 K1 96.769(19) 10 12 ?
K1 Ir1 K1 83.231(19) . 12 ?
K1 Ir1 K1 83.231(19) 10 3 ?
K1 Ir1 K1 180.00(3) . 10 ?
K1 Ir1 K1 180.00(3) 3 12 ?
O1 Ir1 Ir3 130.56(7) 3 10 ?
O1 Ir1 Ir3 49.44(7) 3 . ?
O1 Ir1 Ir3 49.44(7) 2 . ?
O1 Ir1 Ir3 49.44(7) 11 10 ?
O1 Ir1 Ir3 130.56(7) 12 . ?
O1 Ir1 Ir3 49.44(7) 10 10 ?
O1 Ir1 Ir3 49.44(7) . . ?
O1 Ir1 Ir3 49.44(7) 12 10 ?
O1 Ir1 Ir3 130.56(7) 11 . ?
O1 Ir1 Ir3 130.56(7) 2 10 ?
O1 Ir1 Ir3 130.56(7) 10 . ?
O1 Ir1 Ir3 130.56(7) . 10 ?
O1 Ir1 K1 48.12(7) 2 . ?
O1 Ir1 K1 49.86(7) 12 12 ?
O1 Ir1 K1 48.12(7) 10 12 ?
O1 Ir1 K1 109.12(7) 3 . ?
O1 Ir1 K1 70.88(7) 12 . ?
O1 Ir1 K1 131.88(7) 11 . ?
O1 Ir1 K1 130.14(7) 3 12 ?
O1 Ir1 K1 49.86(7) 10 10 ?
O1 Ir1 K1 131.88(7) 2 10 ?
O1 Ir1 K1 130.14(7) 10 . ?
O1 Ir1 K1 109.12(7) 12 10 ?
O1 Ir1 K1 70.88(7) 11 3 ?
O1 Ir1 K1 131.88(7) . 12 ?
O1 Ir1 K1 130.14(7) 12 3 ?
O1 Ir1 K1 109.12(7) 11 12 ?
O1 Ir1 K1 109.12(7) 2 3 ?
O1 Ir1 K1 70.88(7) 2 12 ?
O1 Ir1 K1 130.14(7) . 10 ?
O1 Ir1 K1 70.88(7) 3 10 ?
O1 Ir1 K1 48.12(7) . 3 ?
O1 Ir1 K1 49.86(7) . . ?
O1 Ir1 K1 49.86(7) 3 3 ?
O1 Ir1 K1 48.12(7) 11 10 ?
O1 Ir1 K1 131.88(7) 10 3 ?
O1 Ir1 O1 97.72(10) 3 11 ?
O1 Ir1 O1 180.00(16) 11 2 ?
O1 Ir1 O1 82.28(10) 10 11 ?
O1 Ir1 O1 82.28(10) 10 12 ?
O1 Ir1 O1 180.0(3) 10 . ?
O1 Ir1 O1 97.72(10) . 12 ?
O1 Ir1 O1 82.28(10) 3 2 ?
O1 Ir1 O1 180.00(14) 3 12 ?
O1 Ir1 O1 97.72(10) 12 2 ?
O1 Ir1 O1 82.28(10) 11 12 ?
O1 Ir1 O1 82.28(10) . 3 ?
O1 Ir1 O1 97.72(10) 10 2 ?
O1 Ir1 O1 97.72(10) . 11 ?
O1 Ir1 O1 82.28(10) . 2 ?
O1 Ir1 O1 97.72(10) 10 3 ?
Ir3 Ir2 Ir3 180.0 . 10_556 ?
Ir3 Ir2 K1 88.488(15) . 16 ?
Ir3 Ir2 K1 91.512(15) . 4_445 ?
Ir3 Ir2 K1 91.512(15) . 5 ?
Ir3 Ir2 K1 91.512(15) 10_556 16 ?
Ir3 Ir2 K1 88.488(15) . 17_445 ?
Ir3 Ir2 K1 88.488(15) 10_556 4_445 ?
Ir3 Ir2 K1 91.512(15) 10_556 17_445 ?
Ir3 Ir2 K1 88.488(15) 10_556 5 ?
K1 Ir2 K1 60.068(1) 17_445 4_445 ?
K1 Ir2 K1 119.932(1) 5 4_445 ?
K1 Ir2 K1 119.932(1) 17_445 16 ?
K1 Ir2 K1 180.0 16 4_445 ?
K1 Ir2 K1 60.068(1) 5 16 ?
K1 Ir2 K1 180.0 5 17_445 ?
O2 Ir2 Ir3 131.04(6) 10_556 . ?
O2 Ir2 Ir3 48.96(6) 10_556 10_556 ?
O2 Ir2 Ir3 48.96(6) 11_556 10_556 ?
O2 Ir2 Ir3 131.04(6) . 10_556 ?
O2 Ir2 Ir3 48.96(6) 2 . ?
O2 Ir2 Ir3 131.04(6) 12_556 . ?
O2 Ir2 Ir3 131.04(6) 2 10_556 ?
O2 Ir2 Ir3 131.04(6) 3 10_556 ?
O2 Ir2 Ir3 48.96(6) . . ?
O2 Ir2 Ir3 131.04(6) 11_556 . ?
O2 Ir2 Ir3 48.96(6) 3 . ?
O2 Ir2 Ir3 48.96(6) 12_556 10_556 ?
O2 Ir2 K1 53.82(7) 11_556 5 ?
O2 Ir2 K1 81.08(7) 3 16 ?
O2 Ir2 K1 46.09(7) 11_556 16 ?
O2 Ir2 K1 126.18(7) 2 5 ?
O2 Ir2 K1 53.82(7) 10_556 4_445 ?
O2 Ir2 K1 98.92(7) . 5 ?
O2 Ir2 K1 126.18(7) 10_556 16 ?
O2 Ir2 K1 81.08(7) 10_556 5 ?
O2 Ir2 K1 46.09(7) 2 4_445 ?
O2 Ir2 K1 133.91(7) 12_556 5 ?
O2 Ir2 K1 98.92(7) 3 4_445 ?
O2 Ir2 K1 46.09(7) 3 5 ?
O2 Ir2 K1 53.82(7) . 16 ?
O2 Ir2 K1 126.18(7) 11_556 17_445 ?
O2 Ir2 K1 98.92(7) 12_556 16 ?
O2 Ir2 K1 53.82(7) 2 17_445 ?
O2 Ir2 K1 133.91(7) 11_556 4_445 ?
O2 Ir2 K1 81.08(7) . 17_445 ?
O2 Ir2 K1 126.18(7) . 4_445 ?
O2 Ir2 K1 98.92(7) 10_556 17_445 ?
O2 Ir2 K1 81.08(7) 12_556 4_445 ?
O2 Ir2 K1 46.09(7) 12_556 17_445 ?
O2 Ir2 K1 133.91(7) 3 17_445 ?
O2 Ir2 K1 133.91(7) 2 16 ?
O2 Ir2 O2 81.56(10) 2 . ?
O2 Ir2 O2 98.44(9) 10_556 3 ?
O2 Ir2 O2 98.44(10) . 12_556 ?
O2 Ir2 O2 81.56(10) 11_556 10_556 ?
O2 Ir2 O2 81.56(10) 11_556 12_556 ?
O2 Ir2 O2 98.44(10) 2 10_556 ?
O2 Ir2 O2 180.0 11_556 2 ?
O2 Ir2 O2 180.00(10) . 10_556 ?
O2 Ir2 O2 180.0 12_556 3 ?
O2 Ir2 O2 98.44(10) 11_556 . ?
O2 Ir2 O2 98.44(10) 2 12_556 ?
O2 Ir2 O2 81.56(10) 2 3 ?
O2 Ir2 O2 81.56(10) 10_556 12_556 ?
O2 Ir2 O2 98.44(10) 11_556 3 ?
O2 Ir2 O2 81.56(10) . 3 ?
Ir1 Ir3 Ir2 180.0 . . ?
Ir1 Ir3 K1 76.167(16) . 3 ?
Ir1 Ir3 K1 76.167(16) . . ?
Ir1 Ir3 K1 76.167(16) . 2 ?
Ir2 Ir3 K1 103.833(16) . . ?
Ir2 Ir3 K1 103.833(16) . 3 ?
Ir2 Ir3 K1 103.833(16) . 2 ?
K1 Ir3 K1 114.472(13) 2 . ?
K1 Ir3 K1 114.472(13) 2 3 ?
K1 Ir3 K1 114.472(13) 3 . ?
O1 Ir3 Ir1 48.96(6) 2 . ?
O1 Ir3 Ir1 48.96(6) 3 . ?
O1 Ir3 Ir1 48.96(6) . . ?
O1 Ir3 Ir2 131.04(6) 3 . ?
O1 Ir3 Ir2 131.04(6) . . ?
O1 Ir3 Ir2 131.04(6) 2 . ?
O1 Ir3 K1 57.60(7) 3 2 ?
O1 Ir3 K1 125.11(7) . 2 ?
O1 Ir3 K1 59.32(7) . . ?
O1 Ir3 K1 125.11(7) 3 . ?
O1 Ir3 K1 57.60(7) 2 . ?
O1 Ir3 K1 59.32(7) 2 2 ?
O1 Ir3 K1 125.11(7) 2 3 ?
O1 Ir3 K1 57.60(7) . 3 ?
O1 Ir3 K1 59.32(7) 3 3 ?
O1 Ir3 O1 81.56(10) 3 2 ?
O1 Ir3 O1 81.56(10) . 2 ?
O1 Ir3 O1 81.56(10) 3 . ?
O2 Ir3 Ir1 130.92(6) . . ?
O2 Ir3 Ir1 130.92(6) 3 . ?
O2 Ir3 Ir1 130.92(6) 2 . ?
O2 Ir3 Ir2 49.08(6) . . ?
O2 Ir3 Ir2 49.08(6) 3 . ?
O2 Ir3 Ir2 49.08(6) 2 . ?
O2 Ir3 K1 124.33(7) 2 3 ?
O2 Ir3 K1 118.78(7) 2 . ?
O2 Ir3 K1 118.78(7) 3 2 ?
O2 Ir3 K1 118.78(7) . 3 ?
O2 Ir3 K1 124.33(7) . 2 ?
O2 Ir3 K1 54.86(7) . . ?
O2 Ir3 K1 54.86(7) 2 2 ?
O2 Ir3 K1 54.86(7) 3 3 ?
O2 Ir3 K1 124.33(7) 3 . ?
O2 Ir3 O1 178.06(9) 2 . ?
O2 Ir3 O1 97.08(10) . . ?
O2 Ir3 O1 178.06(9) . 3 ?
O2 Ir3 O1 178.06(9) 3 2 ?
O2 Ir3 O1 99.65(9) . 2 ?
O2 Ir3 O1 97.08(10) 2 2 ?
O2 Ir3 O1 99.65(9) 3 . ?
O2 Ir3 O1 99.65(9) 2 3 ?
O2 Ir3 O1 97.08(9) 3 3 ?
O2 Ir3 O2 81.75(10) . 2 ?
O2 Ir3 O2 81.75(10) 3 2 ?
O2 Ir3 O2 81.75(10) . 3 ?
Ir2 K1 K1 98.98(3) 7_554 6_455 ?
Ir2 K1 K1 80.17(3) 7_554 8_554 ?
Ir2 K1 K1 59.964(1) 7_554 15 ?
Ir2 K1 K1 59.966(1) 7_554 14_455 ?
Ir3 K1 Ir2 134.55(3) . 7_554 ?
Ir3 K1 K1 76.93(3) . 15 ?
Ir3 K1 K1 81.04(3) . 6_455 ?
Ir3 K1 K1 161.06(3) . 14_455 ?
Ir3 K1 K1 119.35(3) . 8_554 ?
K1 K1 K1 109.06(4) 15 6_455 ?
K1 K1 K1 84.57(4) 14_455 6_455 ?
K1 K1 K1 70.94(4) 14_455 8_554 ?
K1 K1 K1 152.30(4) 8_554 6_455 ?
K1 K1 K1 94.58(3) 15 8_554 ?
K1 K1 K1 119.724(5) 15 14_455 ?
O1 K1 Ir2 159.88(5) 2 7_554 ?
O1 K1 Ir2 110.26(6) 14_455 7_554 ?
O1 K1 Ir2 106.33(5) . 7_554 ?
O1 K1 Ir3 38.06(5) 2 . ?
O1 K1 Ir3 37.92(5) . . ?
O1 K1 Ir3 111.07(6) 14_455 . ?
O1 K1 K1 103.55(6) 2 15 ?
O1 K1 K1 133.47(6) 2 14_455 ?
O1 K1 K1 97.49(5) 2 6_455 ?
O1 K1 K1 47.26(5) . 15 ?
O1 K1 K1 90.52(5) 2 8_554 ?
O1 K1 K1 160.79(6) . 14_455 ?
O1 K1 K1 112.15(6) . 6_455 ?
O1 K1 K1 87.75(6) 14_455 8_554 ?
O1 K1 K1 169.20(6) 14_455 15 ?
O1 K1 K1 51.26(6) 14_455 14_455 ?
O1 K1 K1 66.39(6) 14_455 6_455 ?
O1 K1 K1 94.37(5) . 8_554 ?
O1 K1 O1 86.94(8) 14_455 2 ?
O1 K1 O1 56.30(9) 2 . ?
O1 K1 O1 143.16(8) 14_455 . ?
O1 K1 O2 100.21(8) 14_455 . ?
O1 K1 O2 90.12(7) . 16 ?
O1 K1 O2 141.85(7) 2 16 ?
O1 K1 O2 123.21(8) 14_455 16 ?
O2 K1 Ir2 115.94(6) . 7_554 ?
O2 K1 Ir2 34.21(4) 16 7_554 ?
O2 K1 Ir2 33.60(5) 8_554 7_554 ?
O2 K1 Ir3 38.01(5) . . ?
O2 K1 Ir3 104.49(5) 16 . ?
O2 K1 Ir3 146.05(6) 8_554 . ?
O2 K1 K1 130.21(7) . 14_455 ?
O2 K1 K1 81.58(7) . 15 ?
O2 K1 K1 46.25(5) 16 15 ?
O2 K1 K1 52.82(5) 8_554 14_455 ?
O2 K1 K1 77.56(5) 16 6_455 ?
O2 K1 K1 74.31(6) 8_554 15 ?
O2 K1 K1 157.35(6) . 8_554 ?
O2 K1 K1 111.49(6) 16 8_554 ?
O2 K1 K1 45.76(5) . 6_455 ?
O2 K1 K1 125.41(6) 8_554 6_455 ?
O2 K1 K1 46.85(5) 8_554 8_554 ?
O2 K1 K1 84.20(5) 16 14_455 ?
O2 K1 O1 100.01(7) 8_554 14_455 ?
O2 K1 O1 135.83(7) 8_554 2 ?
O2 K1 O1 66.60(8) . . ?
O2 K1 O1 68.98(8) . 2 ?
O2 K1 O1 108.13(7) 8_554 . ?
O2 K1 O2 81.94(8) . 16 ?
O2 K1 O2 148.67(6) 8_554 . ?
O2 K1 O2 66.97(10) 8_554 16 ?
Ir1 O1 Ir3 81.61(8) . . ?
Ir1 O1 K1 99.21(9) . 3 ?
Ir1 O1 K1 97.29(9) . . ?
Ir1 O1 K1 146.56(12) . 15 ?
Ir3 O1 K1 130.79(11) . 15 ?
Ir3 O1 K1 84.34(8) . 3 ?
Ir3 O1 K1 82.76(8) . . ?
K1 O1 K1 81.48(7) 15 . ?
K1 O1 K1 157.31(9) 3 . ?
K1 O1 K1 93.06(8) 15 3 ?
Ir2 O2 K1 100.31(9) . 6_455 ?
Ir2 O2 K1 91.98(8) . 16 ?
Ir2 O2 K1 168.24(11) . . ?
Ir3 O2 Ir2 81.96(8) . . ?
Ir3 O2 K1 152.72(12) . 6_455 ?
Ir3 O2 K1 87.13(8) . . ?
Ir3 O2 K1 126.31(11) . 16 ?
K1 O2 K1 87.39(7) 6_455 . ?
K1 O2 K1 98.06(8) . 16 ?
K1 O2 K1 80.94(6) 6_455 16 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ir1 Ir3 2.6221(3) . ?
Ir1 Ir3 2.6221(3) 10 ?
Ir1 K1 3.6556(8) 10 ?
Ir1 K1 3.6556(8) . ?
Ir1 K1 3.6556(8) 12 ?
Ir1 K1 3.6556(8) 3 ?
Ir1 O1 1.999(2) 11 ?
Ir1 O1 1.999(2) 3 ?
Ir1 O1 1.999(2) 12 ?
Ir1 O1 1.999(2) 2 ?
Ir1 O1 1.999(2) . ?
Ir1 O1 1.999(2) 10 ?
Ir2 Ir3 2.6306(3) . ?
Ir2 Ir3 2.6306(3) 10_556 ?
Ir2 K1 3.5688(8) 5 ?
Ir2 K1 3.5688(8) 16 ?
Ir2 K1 3.5688(8) 17_445 ?
Ir2 K1 3.5688(8) 4_445 ?
Ir2 O2 2.007(2) 11_556 ?
Ir2 O2 2.007(2) 2 ?
Ir2 O2 2.007(2) 12_556 ?
Ir2 O2 2.007(2) . ?
Ir2 O2 2.007(2) 10_556 ?
Ir2 O2 2.007(2) 3 ?
Ir3 K1 3.2500(8) 3 ?
Ir3 K1 3.2500(8) 2 ?
Ir3 K1 3.2500(8) . ?
Ir3 O1 2.014(2) 2 ?
Ir3 O1 2.014(2) 3 ?
Ir3 O1 2.014(2) . ?
Ir3 O2 2.004(2) . ?
Ir3 O2 2.004(2) 3 ?
Ir3 O2 2.004(2) 2 ?
K1 Ir2 3.5688(8) 7_554 ?
K1 K1 3.5726(8) 14_455 ?
K1 K1 3.6438(4) 8_554 ?
K1 K1 3.6438(4) 6_455 ?
K1 K1 3.5725(8) 15 ?
K1 O1 2.817(3) . ?
K1 O1 2.757(2) 2 ?
K1 O1 2.653(2) 14_455 ?
K1 O2 2.882(2) 16 ?
K1 O2 2.613(2) 8_554 ?
K1 O2 2.661(2) . ?
O1 K1 2.757(2) 3 ?
O1 K1 2.653(2) 15 ?
O2 K1 2.613(2) 6_455 ?
O2 K1 2.882(2) 16 ?
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.5956(19)
2 0.4044(19)
